Properties and Applications of Materials Classification of Materials Materials Metals Polymers Ceramics Metals Metals Ferrous Steel and Cast Irons Non-Ferrous Al, Cu, Mg etc. Ferrous Materials Ferrous Steels Low Alloy Stainless steel Cast iron High Alloy Tool steel Ferrous Materials - Steels • Steels - alloys of iron-carbon. May contain other alloying elements. • Several grades are available. • Low Alloy (<10 wt%) –Low Carbon (<0.25 wt% C) –Medium Carbon (0.25 to 0.60 wt%) –High Carbon (0.6 to 1.4 wt%) • High Alloy –Stainless Steel (> 11 wt% Cr) –Tool Steel Steels Low alloy High alloy Low Carbon Stainless Medium Carbon Tool High Carbon Low Carbon Steel Plain carbon steels - very low content of alloying elements and small amounts of Mn. Most abundant grade of steel is low carbon steel - greatest quantity produced; least expensive. Not responsive to heat treatment; cold working needed to improve the strength. Good Weldability and machinability High Strength, Low Alloy (HSLA) steels - alloying elements (like Cu, V, Ni and Mo) up to 10 wt %; have higher strengths and may be heat treated. Low carbon steel Compositions of some low carbon and low alloy steels Properties and typical application of some low carbon and low alloys steels Medium Carbon Steel Carbon content in the range of 0.3 – 0.6%. Can be heat treated - austenitizing, quenching and then tempering. Most often used in tempered condition – tempered martensite Medium carbon steels have low hardenability Addition of Cr, Ni, Mo improves the heat treating capacity Heat treated alloys are stronger but have lower ductility Typical applications – Railway wheels and tracks, gears, crankshafts. Composition of some alloyed medium carbon steels High Carbon Steel High carbon steels – Carbon content 0.6 – 1.4% High C content provides high hardness and strength. Hardest and least ductile. Used in hardened and tempered condition Strong carbide formers like Cr, V, W are added as alloying elements to from carbides of these metals. Used as tool and die steels owing to the high hardness and wear resistance property Compositions and Application of some Tool steels Effects of Alloying Elements on Steel •Manganese – strength and hardness; decreases ductility and weldability; effects hardenability of steel. •Phosphorus – increases strength and hardness and decreases ductility and notch impact toughness of steel. •Sulfur decreases ductility and notch impact toughness Weldability decreases. Found in the form of sulfide inclusions. •Silicon – one of the principal deoxidizers used in steel making. In low-carbon steels, silicon is generally detrimental to surface quality. •Copper – detrimental to hot-working steels; beneficial to corrosion resistance (Cu>0.20%) •Nickel - ferrite strengthener; increases the hardenability and impact strength of steels. •Molybdenum increases the hardenability; enhances the creep resistance of low-alloy steels Stainless steel •Stainless steels - A group of steels that contain at least 11% Cr. Exhibits extraordinary corrosion resistance due to formation of a very thin layer of Cr2O3 on the surface. Categories of stainless steels: Ferritic Stainless Steels – Composed of ferrite (BCC) Martensitic Stainless Steels – Can be heat treated. Austenitic Stainless Steels – Austenite () phase field is extended to room temperature. Most corrosion resistant. Precipitation-Hardening (PH) Stainless Steels – Ultra highstrength due to precipitation hardening. Duplex Stainless Steels – Ferrite + Austenite Composition and Properties of some stainless steels are given in the next slide Applications of Stainless steels Cast Irons Carbon 2.1- 4.5 wt% and Si (normally 1-3 wt%). Lower melting point (about 300 °C lower than pure iron) due to presence of eutectic point at 1153 °C and 4.2 wt% C. Low shrinkage and good fluidity and casting ability. Types of cast iron: grey, white, nodular, malleable and compacted graphite. Grey Cast Iron Grey cast iron contains graphite in the form of flakes. Named after its grey fractured surface. C:3.0 – 4.0 wt%, Si: 1.0 – 3.0 % Microstructure: graphite flakes in a ferrite or pearlite matrix Weak & brittle in tension (the graphite flake tips act as stress concentration sites).Stronger in compression, Excellent damping capacity, wear resistance. Microstructure modification by varying silicon content and cooling rate Casting shrinkage is low Nodular or Ductile Iron Addition of Mg and/or Cerium to grey iron converts the graphite flakes to nodules. Normally a pearlite matrix. Castings are stronger and much more ductile than grey iron as the stress concentration points existing at the flake tips are eliminated. White Cast Iron White cast iron – C: 2.5 – 3 wt.%, Si: 0.5 – 1.5%. Most of the carbon is in the form of cementite. Named after its white fracture surface. Results from faster cooling. Contains pearlite + cementite, not graphite. Thickness variation may result in nonuniform microstructure from variable cooling Very hard and brittle Used as intermediate to produce malleable cast iron. Malleable Cast Iron Malleable cast iron – Carbon: 2.3 – 2.7 wt%, Si: 1.0 – 1.75 % Obtained by heat treating white iron for a prolonged period that causes decomposition of cementite into graphite. Heat treatment : Two stages – Isothermal holding at 950 C and then holding at 720 C. graphite forms in the form of rosettes in a ferrite or pearlite matrix. Reasonable strength and improved ductility (malleable) Heat treatment White iron Malleable Compact Graphite Iron (CGI) CGI graphite occurs as blunt flakes or with a worm-like shape (vermicular). Carbon: 3.1 – 4.0 wt%, Silicon: 1.7 – 3.0 wt %. Microstructure and properties are between gray and ductile iron. Alloying addition may be needed to minimize the sharp edges and formation of spheroidal graphite. Matrix varies with alloy additions or heat treatment. As castable as grey iron, but has a higher tensile strength and some ductility. Relatively high thermal conductivity, good resistance to thermal shock, lower oxidation at elevated temperatures. Applications of Cast iron Cast irons are used in wide variety of application owing to the properties like good fluidity, ease of casting, low shrinkage, excellent machinability, wear resistance and damping capacity. Applications – Car parts – cylinder heads, blocks and gearbox cases. Pipes, lids (manhole lids) Foundation for big machines (good damping property) Bridges, buildings Cook wares – Excellent heat retention Nonferrous Metals • Cu Alloys Brass: Cu-Zn alloy. Corrosion resistant. Used in costume jewelry, coins • Al Alloys -low : 2.7 g/cm3 -Cu, Mg, Si, Mn, Zn additions -solid solution or precipitation Bronze : Cu – with Sn, strengthened (structural Al, Si, Ni aircraft parts & packaging) Cu-Be: • Mg Alloys precipitation hardened Nonferrous -very low : 1.7g/cm3 (bushings, landing gear) -ignites easily -aircraft, missiles • Ti Alloys • Refractory metals relatively low : 4.5 g/cc -high melting T’s Noble metals reactive at high T’s - Ag, Au, Pt -Nb, Mo, W, Ta space and biomedical oxidation/corrosion application resistant Copper Copper is one of the earliest metals discovered by man. The boilers on early steamboats were made from copper. The copper tubing used in water plumbing in Pyramids was found in serviceable condition after more than 5,000 years. Cu is a ductile metal. Pure Cu is soft and malleable, difficult to machine. Very high electrical conductivity – second only to silver. Copper is refined to high purity for many electrical applications. Excellent thermal conductivity – Copper cookware most highly regarded – fast and uniform heating. Electrical and construction industries are the largest users of Cu. Copper The second largest use of Cu is probably in coins. The U.S. nickel is actually 75% copper. The dime, quarter, and half dollar coins contain 91.67% copper and the Susan B Anthony dollar is 87.5% copper. The various Euro coins are made of Cu-Ni, Cu-Zn-Ni or Cu-Al-Zn-Sn alloys. Copper Alloys Brasses and Bronzes are most commonly used alloys of Cu. Brass is an alloy with Zn. Bronzes contain tin, aluminum, silicon or beryllium. Other copper alloy families include copper-nickels and nickel silvers. More than 400 copper-base alloys are recognized. Alloy Family of Cu Alloys Alloying element Brass Zinc (Zn) Phosphor bronze Aluminium bronzes Silicon bronzes Copper nickel, nickel silvers Tin (Sn) Aluminium (Al) Silicon (Si) Nickel (Ni) UNS numbers C1xxxx–C4xxxx,C66400– C69800 C5xxxx C60600–C64200 C64700–C66100 C7xxxx Copper Alloys - Brass Brass is the most common alloy of Cu – It’s an alloy with Zn Brass has higher ductility than copper or zinc. Easy to cast - Relatively low melting point and high fluidity Properties can be tailored by varying Zn content. Some of the common brasses are yellow, naval and cartridge. Brass is frequently used to make musical instruments (good ductility and acoustic properties). Bronze Copper alloys containing tin, lead, aluminum, silicon and nickel are classified as bronzes. Cu-Sn Bronze is one of the earliest alloy to be discovered as Cu ores invariably contain Sn. Stronger than brasses with good corrosion and tensile properties; can be cast, hot worked and cold worked. Wide range of applications: ancient Chinese cast artifacts, skateboard ball bearings, surgical and dental instruments. Bronze bearing Beryllium copper Cu-Be alloys are heat treatable. Max solubility of Be in Cu is 2.7% at 866 C. Decreasing solubility at lower temp. imparts precipitation hardening ability. Cast alloys - higher Be. Wrought alloys – lower Be and some Co Cu-Be is ductile, weldable and machinable. Also resistant to non-oxidizing acids (HCl or H2CO3), abrasive wear and galling. Thermal conductivity is between steels and aluminum. Applications Used in springs, load cells and other parts subjected to repeated loading. Low-current contacts for batteries and electrical connectors. Cast alloys are used in injection molds. Other applications include jet aircraft landing gear bearings and bushings and percussion instruments. Compositions, Properties and Application of some Cu Alloys Name UNS Compos. Condition YS UTS %El Applications No. (wt.%) (MPa) (MPa) Eletrolytic C11000 0.04 O Annealed 69 220 45 Electrical wires, Copper roofing, nails, rivets Cartridge C26000 30.0 Zn Cold435 525 8 Automotive radiator brass rolled core, lamp fixture, ammunition. Phosphor C51000 5.0 Sn, Annealed 130 325 64 Bellows, clutch disk, bronze 0.25 P diaphragm, fuse clips, springs Yellow C85400 29 Zn, As cast 83 234 35 Furniture, radiator bras 3.0 Pb, fittings, battery clamps, (Leaded) 1 Sn light fixtures Al bronze C95400 11 Al, As cast 241 586 18 Bearings, bushings, 4 Fe valve seats and guards Beryllium C17200 1.9 Be Precipita. 965 1140 10 Electrical, valves, copper 0.2 Co hardened pumps Cu - Ni C71500 30 Ni Annealed 125 380 36 Condenser, heatexchanger, piping, valves Tin bronze C90500 10 Sn, As cast 152 310 25 Bearings, bushing, 2 Zn piston rings, gears Aluminum Aluminum is a light metal ( = 2.7 g/cc); is easily machinable; has wide variety of surface finishes; good electrical and thermal conductivities; highly reflective to heat and light. Versatile metal - can be cast, rolled, stamped, drawn, spun, roll-formed, hammered, extruded and forged into many shapes. Aluminum can be riveted, welded, brazed, or resin bonded. Corrosion resistant - no protective coating needed, however it is often anodized to improve surface finish, appearance. Al and its alloys - high strength-to-weight ratio (high specific strength) owing to low density. Such materials are widely used in aerospace and automotive applications where weight savings are needed for better fuel efficiency and performance. Al-Li alloys are lightest among all Al alloys and find wide applications in the aerospace industry. Aluminum Alloys Aluminum alloys are classified into two categories – Cast and Wrought alloys. Wrought alloys can be either heat-treatable or non-heat treatable. Alloys are designated by a 4 digit number. Wrought – the 1st digit indicates the major alloying element. Cast – The last digit after the decimal indicates product from( casting - 0 or ingot -1) As Cast Wrought Alloy Series 1xxx 2xxx 3xxx 4xxx 5xxx 6xxx 7xxx 8xxx Principal Alloying Element Minimum 99.00% Aluminum Copper Manganese Silicon Magnesium Magnesium and Silicon Zinc Other Elements Alloy Principal Alloying Element Series 1xx.x Aluminum, 99.00% or greater 2xx.x Copper 3xx.x Silicon with Copper and/or Magnesium 4xx.x Silicon 5xx.x Magnesium 6xx.x Unused Series 7xx.x Zinc 8xx.x Tin 9xx.x Other Elements Temper Designations F As fabricated - products in which no thermal treatments or strain-hardening. H Strain-hardened (wrought products) – strain hardened with or without additional thermal treatment. H1 Strain-hardened only - strain-hardened without thermal treatment. O Annealed, recrystallized T Thermally treated with or without strain-hardening to produce stable tempers other than F, O or H. T3 Solution heat-treated and then cold worked. Solution heat treatment – heating to the single phase region and isothermal holding. Compositions, Properties and Application of some Al Alloys Al Ass. Composition No (wt.%) 1100 0.12 Cu 3003 5052 2024 6061 7075 359.0 8090 Condition YS UTS %El Applications (MPa) (MPa) Annealed 35 90 45 Food/chemical handling (O) equipment, heat exchangers light reflectors 0.12 Cu,1.2 Annealed 40 110 30 Utensils, pressure vessels and Mn, 0.1 Zn piping 2.5 Mg, 0.25 Strain-hardn. 195 230 14 Bellows, clutch disk, Cr (H32) diaphragm, fuse clips, springs 4.4 Cu, 1.5 Heat treated 325 470 20 Aircraft structure, rivets, truck Mg, 0.6 Mn (T4) wheels, screw 1 Mg, 0.6 Si, T4 145 240 22 Trucks, canoes, railroad cars, 0.3 Cu, 0.2 Cr furniture, pipelines 5.6 Zn, 2.5 Peak-aged 505 570 11 Aircraft structures and other Mg, 1.6 Cu, (T6) highly loaded applications 0.23 Cr 7 Si, 0.3 Mg T6 164 228 4 Aircraft pump parts, automotive transmission cases, cylinder blocks 2.0 Li. 1.3 Heat treated 360 465 Damage tolerant aircraft Cu, 0.95 Mg, cold-worked structures 0.12 Zr (T651) Titanium Pure titanium melts at 1670 oC and has a low density of 4.51 g/cc (40% lighter than steel and 60% heavier than aluminum). Titanium has high affinity to oxygen – strong deoxidiser. Can catch fire and cause severe damage Ti is stronger than Al - high strength and low weight makes titanium very useful as a structural metal. Excellent corrosion resistance due to a presence of a protective thin oxide surface film. Can be used as biomaterial. Can be used in elevated temperature components. Limitation of pure Ti is its lower strength. Alloying is done to improve strength. Titanium Oxygen, nitrogen, and hydrogen can cause titanium to become more brittle. Care should be taken during processing. Titanium can also be cast using a vacuum furnace. Because of its high strength to weight ratio and excellent corrosion resistance, titanium is used in a variety of applications: Aircraft – Body structure, Engine parts sporting equipment, chemical processing, desalination, turbine engine parts, valve and pump parts, marine hardware Medical implants - prosthetic devices. Recently use of Ti in bikes and automotives is increasing Titanium alloys Pure Ti exhibits two phases – Hexagonal -phase at room temperature and BCC -phase above 882 C. Strength of Titanium is improved by alloying. Alloying elements are either or stabilizer. Elements with electron/atoms ratio < 4 – stabilizer (Al, O, Ga), = 4 – neutral (Sn, Zr) and > 4 – stabilizer (V, Mo,Ta, W). ( + ) two-phase alloys can be obtained with right proportions of alloying elements. alloys have low density, moderate strength, reasonable ductility and good creep resistance. Metastable alloys are heavier, stronger and less ductile than alloys. Creep strength reduces with increasing content ( + ) alloys show a good strength-ductility combination Compositions, Properties and Application of some Ti Alloys Alloy Comp . wt.% type (UNS No) CP Ti 99.1Ti (R50500) Ti-5Al-2.5Sn (R54520) Near- Ti-8Al-1Mo1V (R54810) - - Ti-6Al-4V (R56400) Ti-6Al-6V 2Sn (R56620) Ti-10V -2Fe3Al Condition YS UTS %El Applications (MPa) (MPa) Annealed 414 484 45 Airframe skins, marine and chemical processing equipments Annealed 784 826 16 Gas turbine engine casing and rings, chemical processing equipment Annealed 890 950 15 Forged jet engine components – compressor disc, plate, hubs Annealed 877 947 14 Prosthetic implants, airframe components Annealed 985 1050 14 Rocket engine case, airframe structure Heat treated 1150 1223 10 High-strength airframe (aging) components, parts requiring uniform tensile stresses Nickel Nickel is a high-density, high-strength metal with good ductility and excellent corrosion resistance and high temperature properties. Ni has may unique properties including its excellent catalytic property. Nickel Catalyst for Fuel Cells: Nickelcobalt is seen as a low-cost substitute for platinum catalysts. Two-thirds of all nickel produced goes into stainless steel production. Also used extensively in electroplating various parts in variety of applications. Ni-base super alloys are a unique class of materials having exceptionally good high temperature strength, creep and oxidation resistance. Used in many high temperature applications like turbine engines. Nickel Shape Memory Alloys: Ni base (Ni-Ti) and Ni containing (Cu-Al-Ni) shape memory alloys that can go back to original form, are an important class of engineering materials finding widespread use in many applications. Nickel-containing materials are used in buildings and infrastructure, chemical production, communications, energy (batteries: Ni-Cd, Ni-metal hydrides), environmental protection, food preparation, water treatment and transportation. Applications of Nickel Turbine engine Electroplating Batteries Magnesium Magnesium - Lightest among commonly used metals ( 1.7 g/cm3). Melting point is 650 C and it has HCP structure. Is very reactive and readily combustible in air. Can be used as igniter or firestarter. Thermal conductivity is less than Al while their CTE is almost same. Pure Mg has adequate atmospheric resistance and moderate strength. Properties of Mg can be improved substantially by alloying. Favorable atomic size - Can be alloyed with many elements. Most widely used alloying elements are Al, Zn, Mn and Zr. Mg Alloys – Cast, Wrought Wrought alloys are available in rod, bar, sheet, plate, forgings and extrusions. Magnesium Alloys Mg alloys: Impact and dent resistant, have good damping capacity - effective for high-speed applications. Due to its light weight, superior machinability and ease of casting, Mg and its alloys are used in many applications:– Auto parts, sporting goods, power tools, aerospace equipment, fixtures, electronic gadgets, and material handling equipment. Automotive applications include gearboxes, valve covers, alloy wheels, clutch housings, and brake pedal brackets. Compositions, Properties and Application of some Mg Alloys ASTM No Compos. (wt.%) 3.0 Al, 1.0Zn, 0.2 Mn HK31A 3.0Th, 0.6Zr Condition YS UTS %El Applications (MPa) (MPa) Wrought Alloys AZ31B Extruded 200 262 15 Structure and tubing, cathodic protection 200 255 9 ZK60A Strain hard. Annealed Aged 285 350 11 High temp applications (high strength to 315 C) Forging of max strength for aircrafts Cast Alloys 150 230 3 AZ91D 5.5 Zn, 0.45Zr 9.0Al, 0.15 Mn, 0.7 Zn AM60A 9.0Al, 0.13Mn, AS41A 4.3Al, 1.0 Si, 0.35Mn As cast As cast 130 220 6 As cast 140 210 6 Die-cast parts for automobile, luggage and electronic devices Automotive wheels Die-cast parts requiring good creep strength Ceramics Materials Ceramics Refractory Materials Abrasives Glass Advanced Ceramics Refractory Materials Refractory - retains its strength at high temperatures > 500°C. Must be chemically and physically stable at high temperatures. Need to be resistant to thermal shock, should be chemically inert, and have specific ranges of thermal conductivity and thermal expansion. Are used in linings for furnaces, kilns, incinerators, crucibles and reactors. Aluminium oxide (alumina), silicon oxide (silica), calcium oxide (lime) magnesium oxide (magnesia) and fireclays are used to manufacture refractory materials. Zirconia - extremely high temperatures. SiC and Carbon – also used in some very severe temperature conditions, but cannot be used in oxygen environment, as they will oxidize and burn. Composition of some common refractory materials Composition (wt%) Refractory Al2O3 SiO2 MgO Fireclay 25-45 50-70 High-alumina fireclay 90-50 Silica Cr2O3 Fe2O3 CaO TiO2 %Porosity 0-1 0-1 0-1 1-2 10-25 10-45 0-1 0-1 0-1 1-4 18-25 0.2 96.3 0.6 Periclase 1.0 3.0 90 0.3 Periclase chrome ore 9.0 5.0 73 8.2 2.2 25 3.0 2.5 22 2.0 2.2 21 Advanced Ceramics: Automobile Engine parts Advantages: Operate at high temperatures – high efficiencies; Low frictional losses; Operate without a cooling system; Lower weights than current engines Disadvantages: Ceramic materials are brittle; Difficult to remove internal voids (that weaken structures); Ceramic parts are difficult to form and machine Potential materials: Si3N4 (engine valves, ball bearings), SiC (MESFETS), & ZrO2 (sensors), Possible engine parts: engine block & piston coatings Microelectromechanical systems (MEMS) MEMS – These micron-sized structures such as beams, cantilevers, diaphragms, valves, plates and switches that can function as tiny sensors and actuators. Fabricated by integrated circuit (IC) manufacturing processes: bulk and surface micromachining. Thousands of micromachines can be fabricated on a single silicon wafer with supporting circuits integrated on the chip. Can be massproduced in the millions at low prices. Low-cost, commercial MEMS devices developed for: Corrosion detectors and monitors; Instrumentation for automotive and aerospace; Biological and medical devices; Chemical and environmental sensors; Manufacturing and process control devices ;Virtual reality systems Abrasive Ceramics Abrasives are used in cutting and grinding tools. Diamonds - natural and synthetic, are used as abrasives, though relatively expensive. Industrial diamonds are hard and thermally conductive. Diamonds unsuitable as gemstone are used as industrial diamond Common abrasives – SiC, WC, Al2O3 (corundum) and silica sand. Either bonded to a grinding wheel or made into a powder and used with a cloth or paper. Silicon carbide Glass Glass - inorganic, non-crystalline (amorphous) material. Range - soda-lime silicate glass for soda bottles to the extremely high purity silica glass for optical fibers. Widely used for windows, bottles, glasses for drinking, transfer piping and receptacles for highly corrosive liquids, optical glasses, windows for nuclear applications. The main constituent of glass is silica (SiO2). The most common form of silica used in glass is sand. Sand fusion temp to produce glass - 1700 °C. Adding other chemicals to sand can considerably reduce the fusion temperature. Sodium carbonate (Na2CO3) or soda ash, (75% SiO2 + 25% Na2O) will reduce the fusion temperature to 800 °C. Other chemicals like Calcia (CaO) and magnesia (MgO) are used for stability. Limestone (CaCO3) and dolomite (MgCO3) are used for this purpose as source of CaO and MgO. Key Properties of Glass • Glass-ceramic materials should have: Relatively high mechanical strengths Low coefficients of thermal expansion Relatively high temperature capabilities Good dielectric properties Good biological compatibility Thermal shock resistance Compositions and Characteristics of some common Glasses Polymers Polymers – Chain of H-C molecules. Each repeat unit of H-C is a monomer e.g. ethylene (C2H4), Polyethylene – (–CH2 – CH2)n Polymers: Thermosets – Soften when heated and harden on cooling – totally reversible. Thermoplasts – Do not soften on heating Plastics – moldable into many shape and have sufficient structural rigidity. Are one of the most commonly used class of materials. Are used in clothing, housing, automobiles, aircraft, packaging, electronics, signs, recreation items, and medical implants. Natural plastics – hellac, rubber, asphalt, and cellulose. Characteristics and Applications of some common Thermoplastics Material Characteristics Applications Polyethylene Chemically resistant, tough, low Flexible bottles, toys, battery parts, friction coeff., low strength ice trays, film wrapping materials Polyamide (Nylon) Good strength and toughness, abrasion resistant, liquid absorber, low friction coeff. Bearings, gears, cams, bushings and jacketing for wires and cables Fluorocarbon (Teflon) Chemically inert, excellent electrical properties, relatively weak Anticorrosive seals, chemical pipes and valves, bearings, anti-adhesive coatings, high temp electronic parts Polyester (PET) Tough plastic film, excellent fatigue and tear strength, corrosion resistant Recording tapes, clothing, automotive tyre cords, beverage containers Vinyl Low-cost general purpose material, rigid, can be made flexible Floor coverings, pipe, electric al wire insulation, garden hose, phonograph records Polystyrene Excellent electrical prop and Wall tile, battery cases, toys, lighting optical clarity, good thermal and panels, housing appliances dimensional stability Characteristics and Applications of some common Thermosetting Polymers Material Characteristics Applications Epoxy (Araldite) Excellent mechanical properties and corrosion resistance, good electrical prop., good adhesion and dimensional stability Electrical moldings, sinks, adhesives, protective coatings, fiber reinforced plastic (FRP), laminates Phenolic (Bakelite) Excellent thermal stability (>150C), inexpensive, can be compounded with many resins Motor housings, telephones, auto distributors, electrical fixtures Polyester (Aropol) Excellent electrical properties, low cost, can formulated for room or high temperature, often fiber reinforced Helmets, fiberglass boats, auto body components, chair fans Elastomers Elastomer – a polymer with rubber-like elasticity. Each of the monomers that link to form the polymer is usually made of carbon, hydrogen, oxygen and/or silicon. Cross-linking in the monomers provides the flexibility. Glass transition temperature, Tg, is the temperature at which transition from rubbery to rigid state takes place in polymers. Elastomers are amorphous polymers existing above their Tg. Hence, considerable segmental motion exists in them. Their primary uses are in seals, adhesives and molded flexible parts. Characteristics and Applications of some commercial Elastomers Material Characteristics Applications Natural rubber (NR) Useful temp. range : - 60 – 120Cgood resistance to cutting abrasion, resistant to oil, ozone, elng. 500- 700% Pneumatic tyres and tubes, heels and soles, gaskets Styrenebutadiene copolymer (SBR)) Temp. range: - 60 – 120 C, Good physical properties, elongation 450 – 500% Same as natural rubber Acrylonitrilebutadiene copolymer (NBR) Temp. range: - 50 – 150 C. Excellent resistance to oils, elongation 400 – 600% Gasoline, chemicals and oil hose, seals and O-rings, soles and heels Chloroprene (CR) Temp. range: - 50 – 105 C. Excellent resistance to high and low temp. excellent electrical prop. Elng. 100 – 800% High and low temp. insulation, seals, diaphragm, tubing for food and medical uses Liquid Crystal Polymers (LCP) LCPs are a group of chemically complex structure having unique properties. Primarily used in LCDs (liquid crystal displays) on watches, flat panel computer monitors, televisions and clocks. Advantages - LCDs are thinner and lighter and consume much less power than cathode ray tubes (CRTs). The name "liquid crystal" arises out of their characteristics. It takes a fair amount of heat to change a suitable substance from a solid into a liquid crystal, and it only takes a little more heat to turn the liquid crystal into a real liquid. LCDs use these liquid crystals because they react predictably to electric current in such a way as to control light passage. A particular sort of nematic liquid crystal, called twisted nematics (TN), is naturally twisted. Applying an electric current to these liquid crystals will untwist them to varying degrees, depending on the applied electrical potential. Advanced Polymers Ultrahigh Molecular Weight Polyethylene (UHMWPE) Molecular weight ca. 4 x 106 g/mol Outstanding properties high impact strength resistance to wear/abrasion low coefficient of friction self-lubricating surface Important applications bullet-proof vests golf ball covers hip implants (acetabular cup) UHMWPE References http://www.titaniuminfogroup.co.uk/tech-data-links.php http://www.msm.cam.ac.uk/phase-trans/ 2004/titanium/ titanium.html http://www.nickelinstitute.org/NickelUseInSociety/ http://www.keytometals.com/Article58.htm http://www.alcotec.com/us/en/solutions/-Understanding-theAluminum-Alloy-Designation-System.cfm http://www.efunda.com/materials/alloys/aluminum/temper.cfm http://www.howstuffworks.com/lcd.htm Key words: Application of materials, Ferrous and Noferrous alloys, Stainless steel, Cast iron, aluminium alloys, temper designation, titanium, nickel, magnesium, ceramics, polymers Quiz 1. Classify materials. Classify metals. 2. What are the typical grades of steel? What is the effect of different alloying elements in steel? 3. Why are tool steels hard? What is HSLA steel? 4. What are the major alloying elements in stainless steels? Why are stainless steels resistant to corrosion? 5. What is 17-7PH steel? What is the source of high strength in these steels? 6. What should be minimum carbon content in a cast iron? 7. Why is grey cast iron so brittle? Why is it resistant to wear? 8. How can the ductility of cast irons be increased? 9. What is the shape of graphite in malleable cast iron? 10. What are the useful properties of cast iron? 11. Why is copper used extensively in electrical and thermal applications? Quiz 12. What is Brass? What are typical alloying elements in bronze? 13. Which is the heat treatable alloy of copper? 14. How are Alumium alloys classified and designated? 15. What are the different temper designation of aluminum alloys? 16. Why is titanium resistant to corrosion? 17. What are the typical phases in Ti alloys? What is and stabilizer? 18. Why Ti alloys are preferred for high temperature applications? 19. What are the different categories of ceramic materials? 20. What are the main constituents in refractory ceramics? What are the main constituents of glass? 21. What are the key properties of glass-ceramics? Quiz 22. What are thermosets and thermoplasts? 23. Why do plastics find widespread applications? 24. What is elastomer? What are their typical characteristics and applications? 25. What is glass transition temperature? 26. What is UHMWPE polymer? 27. What is LCP? 28. Why are LCPs used in LCD displays? 29. What is twisted nematics? 30. Name some natural plastics.